FSC 7530 JCP F10
MANIFOLD, WHITE AND COLORED
Manifold Paper February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For offset printing, generally face only, of multiforms and for multiple copies of correspondence. Light weight, low bulk, and low opac-
ity. Printed matter may include text and light line illustrations.
Unless the option below is specified, the following ‘basic’ specification applies.
Stock: 100 pct chemical pulp. Color: The paper in the order (or publication) shall be uniform
Note: 1 Postconsumer fiber, in any percentage, is encouraged, with a target brightness of 79 pct for the white paper. The color
provided that the requirements of this Standard are met. variation shall not exceed DE(CIELAB)=1.0.
For colored stock, paper shall match one of the established
Grammage (g/m 2) .............................................................. 35 standards. Standards are blue, green, pink, salmon, or yellow.
Basis weight: 17 by 22 inches, 500 sheets (pounds) ...... 9 Colors shall not fade and shall appear even and uniform on the
surface of the sheet. Stock shall not be 2-sided. Color coordinates
A tolerance of ±5 pct shall be allowed. for selected standards are included in Part 3.
Bursting strength: Average, not less than (kPa) ........... 50 Finish and formation: Shall be uniform.
Equivalent (lb/in 2) ........................................................... 7 Cleanliness: The dirt count for each side of the paper shall not
Writing quality: Characters written with ball point and felt tip exceed 250 specks per square meter. No sample sheet (600 to
650 cm2 in size) shall contain more than one defect with an
pens shall be clear cut and free from excessive feathering. equivalent area of 0.25 mm2 or greater.
General appearance: Paper shall conform to the standard sam- Sampling and testing: Shall be conducted in accordance with
ple(s) adopted by the Government. standards in Part 2, Government Paper Specification Standards.
Option A: Alkaline paper. This option is for products requiring above average permanence for white stock only.
The following requirements replace the same in the ‘basic’ specification and are added to the specification.
Stock: 100 pct bleached chemical woodpulp. Acidity: pH value by cold extraction shall be not less than 7.0.
The paper shall contain not less than 2 pct calcium carbonate.
Note: Postconsumer fiber, in any percentage, is encouraged, Any deviation in this requirement shall be sufficient cause for
provided that the requirements of this Standard are met. rejection of the paper.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Sizing: Paper shall be surface- and internal-sized suitable for sat- smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16
isfactory printing on both sides of the paper on high-speed offset inch) shall be allowed except for sheets 216 by 356 mm (81⁄2 by
presses equipped with continuous flow or brush dampening sys- 14 inches) or less; then a tolerance of ±1 mm (1⁄32 inch) shall be
tems. allowed. Successive sheets within any package shall not differ
Color: Shall match the Government’s standard sample for color. from each other by more than 0.5 mm (1⁄64 inch). Paper with the
A deviation of DE(CIELAB)±3.0 from the color standard for long dimension 813 mm (32 inches) or less shall be considered
white and 2.0 for colored stocks is allowed. A color difference 1.0 square if the variation does not exceed 1 mm (1⁄32 inch); over
DE unit between felt and wire sides is permitted. 813 mm (32 inches), 2 mm (1⁄16 inch).
Curl: Paper shall lie flat with either no tendency to curl or with Grain: Direction of the grain on flat paper shall be as ordered.
a curl which can be overcome under reasonable working condi-
tions. Pressroom conditions: The bulk of this paper will be used in
Size and trim: Sheets: Paper shall be furnished in the size(s) or- air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
dered and shall be flat, trimmed square on four sides with clean ±8 pct relative humidity.
1 This grade is typically a low Government usage paper and currently not readily and/or economically available with postconsumer
fiber content. If a postconsumer fiber content is desired in the paper, that number will be stated in the procurement document.